Designation: D – 07Standard Guide for Painting Inspectors (Metal Substrates)1 This. Buy ASTM D GUIDE FOR PAINTING INSPECTORS (METAL SUBSTRATES) from SAI Global. ASTM D – Designation: D – 00 Standard Guide for Painting Inspectors (Metal Substrates.
|Published (Last):||1 January 2004|
|PDF File Size:||6.34 Mb|
|ePub File Size:||2.51 Mb|
|Price:||Free* [*Free Regsitration Required]|
NOK 1 ,00 excl.
Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM Headquarters. It includes the key elements of surface asmt, coatings application, and? Where emulsion cleaners, soaps, or detergents are used, they should be removed completely by washing with clean hot water. Reblasting will be necessary on any surface if rust wstm forms before coating can be applied.
It is very important to record and retain test results.
This ensures that you are always up-to-date and saves you both time and money. Roller covers are available in a variety of diameters, lengths, types of fabric, and? Surfaces that have been dry blasted should be brushed with clean brushes, blown with compressed air free of oil and moisture, asgm vacuum cleaned to eliminate any traces of blast products, dust, or dirt from the surface. Replica tape or surface pro? The standard is used by the inspector to assist in determining whether the degree of surface preparation speci?
Vapor degreasing has the advantages over solvent wiping in that hot solvents are used and the solvent condensation removes oils without recontamination. The minimum treatment for aluminum is Type B, Method 3 of Practices Dwhich describes the use of an alcoholic phosphoric acid cleaner.
Relative Humidity and Dew Point. Originally published as D — Runs, sags, or curtains should be brushed out. If painting is done outside, the cleaned areas should receive the? Most obvious is noncompliance with the speci? Surface cleaning power tools consist of non-woven abrasive wheels and discs, coated abrasive discs or sanding pads, coated abrasive? Any thin spots or areas missed in the application should be repainted and permitted to dry before the next coat is applied.
Pinhole and holiday detectors are either low voltage or high voltage. Water may be injected into the air stream to control dust. Astmm impact tools should be kept sharp. Alternatively, the surface may be allowed to weather a minimum of 6 months before cleaning and painting. Maintenance of record book containing all transacations between the inspector and the contractor is essential to eliminate contract disputes.
The difference between the full and the empty weights divided by 10 is the weight in pounds of 1 gal of the paint. All oil, grease, weld? This asm is very brittle and can crack or loosen due to temperature changes d32766 in fabricating and weathering in the?
The contaminants should be removed not simply spread out by a thorough wiping of the affected areas with cloths saturated with clean solvent. Power Tool Cleaning to Bare Metal.
Sieve analysis and visual observation 2. It is the adtm of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
ASTM D – 07 Standard Guide for Painting Inspectors (Metal Substrates)
The cross-cut test, Test Method Dis more reproducible. If it is suspected that the temperature v3276 humidity conditions are such that moisture is condensing upon the surface, measure the relative humidity and dew point as described in Recycled abrasive test 4. Relative humidity is usually an indicator of condensing conditions and speci?
Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. When surface preparation and painting are carried on indoors, overnight delays between coating and painting may be permissible except on blastcleaned surfaces.
Drying and Curing Times. Record coatings batch numbers mixing procedure 9. Product MSD sheets 3. Material Safety Data Sheets needed to ensure that personnel take necessary precautions in handling hazardous materials. Film thickness gages Dry blast cleaning operations should not be conducted on surfaces that will be wet after blasting and before painting. However, it may take 3 or 4 months to harden to be satisfactorily overcoated with a vinyl coating or other type of coating containing strong d32276.
Material is considered tightly adherent if it cannot be lifted with a dull putty knife. Emulsions, cleaning compounds, steam cleaning, or similar methods and materials may also be used. Type and size abrasive 2.
Within the limitations of the composition of the coating, this may be satisfactory, depending upon the type of coating and providing the surface is dry. See Guide D for establishing procedures to certify inspectors for coatings work in nuclear facilities. C Pictorial Standard Sa 2 shows mill scale and con?
ASTM D – 15e1 Standard Guide for Painting Inspectors (Metal Substrates)
As the contents warm up, the excess escapes through the hole and is removed. In use, the cup is? The testers measure the force required to remove a metal stud that has been cemented to the coated surface.